Download presentation

Presentation is loading. Please wait.

Published byJavon Westfield Modified about 1 year ago

1
Asphalt Rubber Mixture Design ADOT’s AR-ACFC and ARAC

2
AR-ACFC Mix Design Considerations

3
AR-ACFC: Purpose Final wearing surface Typically nominal 1/2 inch lift

4
AR-ACFC: Aggregate Gradation Flakiness Sand Equivalent Crushed Faces Abrasion Percent Carbonates

5
AR-ACFC: Gradation

6
AR-ACFC: Mineral Admixture 1% Lime or Cement is mandatory

7
AR-ACFC: Flakiness Maximum Flakiness = 25 To insure good particle shape, and minimize particle breakage.

8
AR-ACFC: Sand Equivalent Minimum 55 To insure that there are not excessive amounts of clay in the aggregate Done on washed aggregate

9
AR-ACFC: Crushed Faces Minimum 95% Single Crushed Faces To insure good particle interlock and good frictional characteristics

10
AR-ACFC: Abrasion Maximum at 100 rev. 9 at 500 rev. 40 To insure that the aggregate will hold up to the wear and tear of traffic

11
AR-ACFC: Percent Carbonates Maximum 30% To minimize the amount of limestone which has a tendency to polish under traffic.

12
AR-ACFC: Mix Design Steps Prepare Aggregate Determine aggregate specific gravities Determine maximum theoretical specific gravity Check draindown Determine mix density

13
AR-ACFC: Design Determine aggregate specific gravities for fine and coarse mineral aggregate Calculate combined specific gravities (oven dry, saturated surface dry, apparent)

14
AR-ACFC: Design Determine the maximum theoretical specific gravity (Rice test) Done at 3.5 to 4.0% binder content Determine the amount of asphalt absorption.

15
AR-ACFC: Design Calculate Binder content: ((.38)(W) + 8.6)(2.620/C)= Binder content W=% water absorption C=combined oven dry specific gravity

16
AR-ACFC: Design Check Draindown using the Schellenberg test This test is performed in the laboratory in order to determine whether or not an unacceptable amount of binder drains down from the mix.

17
AR-ACFC: Design 1. Place Mix in a beaker 2. Place beaker in oven for 1 hour 3. Empty beaker 4. Determine % mass loss

18
AR-ACFC: Design Based on the results of the draindown test, adjust binder content if necessary

19
AR-ACFC: Design Determine mix density –Compact in Forney (4” diameter, 200 psi) –Determine density by volumetrics Information used for determining spread, may also calculate voids for information only

20
AR-ACFC: Typical Design Typically 2 stockpiles: 95% intermediates, 5% fines Typical binder content % (general range %) Over PCC add 1% to design binder content

21
ARAC Mix Design Considerations

22
ARAC: Purpose Highly flexible lift High quality structural lift Typically nominal 2 inch lift

23
ARAC: Aggregate Gradation Sand Equivalent Crushed Faces Abrasion

24
ARAC: Gradation

25
ARAC: Mineral Admixture 1% Lime or Cement is mandatory

26
ARAC: Sand Equivalent Minimum SE=55 To ensure that there are not excessive amounts of clay particles on the aggregate Done on washed aggregate

27
ARAC: Crushed Faces Minimum 95% Single Crushed Faces To insure good particle interlock

28
ARAC: Abrasion Maximum at 100 rev. 9 at 500 rev. 40 To insure that the aggregate will hold up to the wear and tear of traffic

29
ARAC: Mix Design Steps Prepare Aggregate Determine aggregate specific gravities Determine maximum theoretical specific gravity Compact mix, determine optimum binder content Check mix volumterics

30
ARAC: Design Determine aggregate specific gravities for fine and coarse mineral aggregate Calculate combined specific gravities (oven dry, saturated surface dry, apparent)

31
ARAC: Design Determine the maximum theoretical specific gravity (Rice test) Done at 6.0% binder content and calculated to other binder contents as needed

32
ARAC: Design Compact with Marshall hammer at three binder contents Typically 6.5, 7.5, 8.5 or 6.0, 7.0, 8.0 depending on aggregate source Mix/Compact at 325°F

33
ARAC: Design Check Volumetrics, select optimum binder content. Minimum VMA 19.0% Effective Voids % Maximum 1% binder absorption

34
ARAC: Design Watch to make sure that the VMA is not being created by the binder Typically when VMA is being created by the binder, voids will drop VMA/Voids are very interrelated for this mix type

35
ARAC: Design If necessary, adjust gradation to improve VMA or voids. Repeat compaction process and remeasure maximum theoretical specific gravity.

36
ARAC: Typical Design Typical binder content % depending on aggregate source and gradation

37
Thank you

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google